The energy spectrum and the electrical conductivity of ... › publication › fulltext › The-energ... › publication › fulltext › The-energ...by SP Repetsky · 2020 · Cited by 1 — conductivity is zero, and the metal-dielectric transition occurs. If the Fermi l
The energy spectrum and the electrical conductivity of graphene with substitution impurity S.P. Repetsky1 , I.G. Vyshyvana1 , S.P. Kruchinin2 , R.M. Melnyk3 , A.P. Polishchuk4
arXiv:2003.02084v1 [cond-mat.str-el] 4 Mar 2020
1 Institute of High Technologies, Taras Shevchenko National University of Kyiv,
4-g Academician Glushkov Ave., 03022 Kyiv, Ukraine 2 Bogolyubov Institute for Theoretical Physics of the National Academy of Sciences of Ukraine,
14-b Metrolohichna St., 03143 Kyiv, Ukraine 3 National University of Kyiv-Mohyla Academy, 2 Skovorody St., 04070 Kyiv, Ukraine 4 Aerospace Faculty, National Aviation University, 1 Kosmonavta Komarova Ave., 03058 Kyiv, Ukraine
Received August 28, 2019, in ﬁnal form November 25, 2019 The effect of substitution atoms on the energy spectrum and the electrical conductivity of graphene was investigated in a Lifshitz one-electron tight-binding model. It is established that the ordering of impurity atoms results in a gap in the energy spectrum of electrons whose width depends on the order parameter and on the magnitude of the scattering potential. It is shown that if the order parameter is close to its maximum value, there are peaks associated with localized impurity states on the energy curve of the electron states density at the edges of the energy gap. At the electron concentration at which the Fermi level enters the gap region, the electrical conductivity is zero, and the metal-dielectric transition occurs. If the Fermi level falls in the region of the energy band, the electron relaxation time and electrical conductivity tend to inﬁnity when the order parameter reaches its maximum value. The analytical calculations of the electron density and of the electrical conductivity of graphene, made in the limiting case of weak scattering, are compared with the results of the numerical calculations for different scattering potentials. Key words: graphene, energy gap, density of states, ordering parameter, Green’s function, metal-insulator transition
1. Introduction Lately, the possibility of a targeted modification of graphene with the help of purposely-introduced impurities, created defects, and atoms or chemical functional groups deposited on a surface has attracted a particular attention. In this case, broad potentialities for a change in the physical properties of graphene open up due to the controlled introduction of impurities using the method of ionic implantation. Thus, graphene becomes a basis generating a new class of functional materials. Such materials sometimes find unexpected applications in nanoelectromechanical systems, systems of accumulation of hydrogen, etc. Surely, the main hopes are laid on graphene in connection with the expectation that in the nearest future it has all capabilities of becoming a successor of silicon in electronic devices, which permits to significantly increase the level of miniaturization and working frequencies thereof. The quasirelativistic spectrum of charge carriers underlines the uniqueness of graphene, but hampers, at the same time, the use of graphene in field transistors due to the absence of a gap in its spectrum. It is known that the impurities can induce the appearance of a gap in the energy spectrum. The width of the gap depends on the type of impurities and their concentration. Most studies of the energy spectrum of graphene are based on the density functional theory. The most significant achievements are related to the self-consistent meta-gradient approximation and to the method of projection of adjoint waves  realized in the VASP and GAUSSIAN softwares . The numerical calculations executed by this method showed the opening of a gap in the energy spectrum of graphene This work is licensed under a Creative Commons Attribution 4.0 International License . Further distribution of this work must maintain attribution to the author(s) and the published article’s title, journal citation, and DOI.
S.P. Repetsky et al.
caused by the presence of an impurity. However, clarification of the nature of this effect requires, in addition to the mentioned numerical calculations, the analytical studies of the influence of impurities on the energy spectrum and on the properties of graphene. The electronic structures of the isolated monolayer of graphene, two- and three-layer graphenes and graphene grown on ultrathin layers of hexagonal boron nitride (h-BN) were calculated in  within the framework of the density functional theory with the use of the method of pseudopotential. It was shown that the energy gap 57 meV in width appears in the graphene grown on a monolayer of h-BN. Graphenes with impurities of aluminium, silicon, phosphorus, and sulphur were studied within the analogous method in work , where it was shown, in particular, that graphene with a 3% impurity of phosphorus has a gap 0.67 eV in width. In work  with the use of the QUANTUM-ESPRESSO software, the possibilities of the opening of a gap in the energy spectrum of graphene at the introduction of the impurities of boron and nitrogen (the gap width is 0.49 eV), as well